Osseointegration of TI6Al4V dental implants modified by thermal oxidation in osteoporotic rabbits
© The Author(s). 2016
- Received: 2 April 2016
- Accepted: 7 July 2016
- Published: 21 July 2016
In this work, the effect of the heat treatment on Ti6Al4V implants and topical administration of growth hormone to address a better osseointegration in osteoporotic patients has been analysed.
The osseointegration process of Ti6Al4V implants modified by oxidation treatment at 700 °C for 1 h and the influence of local administration of growth hormone (GH) in osteoporotic female rabbits after 15 and 30 days of implantation have been studied. Bone response was analysed through densitometric and histomorphometric studies. Characterization of the surface was provided by scanning electron microscopy.
The oxidation treatment promotes the formation of an oxide scale grown on the Ti6Al4V implants that alters the nanoroughness of the surface. Bone mineral density (BMD) increases from 0.347 ± 0.014 (commercial) to 0.383 ± 0.012 g cm−2 (modified), and bone-to-implant contact (BIC) goes from 48.01 ± 14.78 (commercial) to 55.37 ± 15.31 (modified) after 30 days of implantation.
The oxidation treatment on the Ti6Al4V dental implants enhances the early bone formation at the longest periods of implantation. No significant differences in the BMD and BIC results in healthy and osteoporotic rabbits were revealed with respect to the local administration of GH in the implantation site.
- Growth hormone
- In vivo
- Oxidation treatment
The metallic biomaterials used in the substitution of hard tissues are subjected to the action of the physiological environment and mechanical efforts like fatigue, wear or friction that alter the operation success of implants and affect drastically the electrochemical properties of the surface. That is the case of Ti and its alloys, in which in vivo conditions alter the stability of the passive layer and provoke the release of both metallic ions and particles .
The search for new treatments that increase the wear resistance, improve the bioactivity in order to facilitate the formation of bone tissue around it and decrease the titanium release is increasingly important. Among them, thermal oxidation treatments aimed to obtain “in situ” ceramic coatings can offer thick, highly crystalline oxide films with very good protective performances [2, 3]. The authors have proved that oxidation treatments of Ti6Al4V alloy at 700 °C for 1 h provoke the formation of an oxide layer, mainly composed of rutile  whose ion release is reduced to the half . In vitro experiments with primary osteoblasts cell culture revealed that the surface modification does not alter even improve the excellent biocompatible behaviour. In fact, cell adhesion is favoured on the thermally treated surfaces . However, in vivo evidences have not been previously studied by the authors. At the same way, sandblasting of Ti6Al4V alloys in order to increase the roughness and subsequent thermal treatment improves the osteoblast response. The enhancement of the osseointegration process can be achieved modifying the quality of the surface of the implant in terms of chemical, physical and topographical properties, all of them influencing the functional activity of cells around the implant surface.
On the other hand, in those cases where there is a delay in the physiological mechanisms of bone repair, either by aging or due to problems of osteoporosis, the solution must be taken by means of external substances that stimulate the bone metabolism. Patients diagnosed with systemic diseases such as osteoporosis and diabetes are considered to be medically compromised for implant therapy. Research has been focused on the local application of substances on the implant surface [7–9], or directly in the implantation site, able to accelerate the osseointegration process. Hormones [10–12], growth factors [13, 14] and osseoconductive proteins  are being used to stimulate the bone growth. Studies carried out by Becker et al.  revealed that local application of diverse growth factors (IGF-I and PDGF) induce the statistical increase in bone repair and the increase of bone density, around Ti implants, compared with the control group. Numerous studies highlight the importance of the growth hormone (GH) in the repair of bone fractures as young as old animals. The administration is able to increase up to 400 % the mechanical properties with respect to the control group [17, 18], stimulate the osteoblast activity and enhance the bone neoformationa around implants .
The aim of this study is to study the influence of the thermal treatment of Ti6Al4V dental implants and topical administration of growth hormone on the osseointegration process of osteoporotic rabbits during the first month of implantation.
Implant preparation and characterization
Threaded commercial titanium alloy implants (3.3 mm diameter and 8 mm length) from Zimmer® were used as control implants. They consisted of Ti6Al4V screws blasted with hydroxyapatite and subsequent acid attack with HCl. Screws with these prior surface treatments were submitted to a thermal treatment. The oxidation treatment was performed at 700 °C for 1 h, in air. After oxidation, samples were removed from the furnace and cooled at room temperature. Commercial and heat-modified screws were gamma-ray sterilized prior to implantation.
Scanning electron microscope (SEM) was used to characterize the surface morphology of the Ti implants. The surfaces were analysed by using a JEOL-6500F microscope equipped with a field emission gun (FEG) coupled with an energy dispersive X-ray (EDX) spectrometer. The images were taken using secondary electrons.
Animals and treatment
The experimental protocol of this study and animal care conformed to the European Communities Council Directive of 24 November 1986 (86/609/EEC)  and has been independently reviewed and approved by the Madrid Community Ethics Committee for Regional Clinical Research (CEIC-R). Forty New Zealand female rabbits of approximately 5 kg and 11 months old were chosen as experimentation animals.
Animals were divided into healthy non-ovariectomised group and ovariectomised (OVX) group to carry out the tests. In order to induce osteoporosis, female rabbits underwent bilateral ovariectomy under general anaesthesia and were fed a hypocalcic diet (8.2 g kg−1 calcium and 6 g kg−1 phosphorous) for 8 weeks . Diet mainly consisted of 74.2 % barley, 20 % wheat bran, 5 % soy and 0.3 % salt was supplied by PanLab SL (Harvard Bioscience Group, Barcelona, Spain). This procedure was selected because the treatment based only on the ovariectomy and hypocalcic diet provokes spontaneous fractures [21, 22].
Eight weeks post-surgery, rabbits were subjected to a densitometry to the vertebral column and tibia bone to verify the establishment of osteoporosis model . For the densitometric analysis, a Norland XR-26 densitometer was used (Norland Co., Fort Atkinson, WI, USA) calibrated prior to the measurement. The exploration parameters were as follows: speed 40 mm s−1, resolution 1.0 × 1.0 mm, and measurement resolution 0.5 × 0.5 mm. Forty percent of the total length of each bone was analyzed, including metaphysis and diaphysis regions to verify differences between bone mass of healthy and osteoporotic groups. The value obtained was the bone mineral density (BMD) in grammes per centimetre.
Implant procedure. Surgery
The injury was sutured with absorbable material after the implantation. Antibiotics and anti-inflammatory agents were delivered in the postoperative period to prevent infection and pain. Rabbits were sacrificed after 15 and 30 days of implantation by intravenous injection of 0.4 mg sodium pentobarbital (Dolethal®, Vetoquinol, Cedex, Francia) diluted in serum (Fig. 1).
Tibiae were cleaned from soft tissues to determine the bone mineral density (BMD). Densitometries at 0.5 mm above and 0.5 mm below the Ti6Al4V implant were acquired to compare the BMD of control and OVX groups.
Histological study of each tibia (including the Ti6Al4V implant) for control and modified implants and with and without GH was carried out. Clean hard tissues were fixed in 10 % pH 7 buffered formaldehyde and dehydrated in grading alcohol concentrations. Tibiae were cut into blocks and histologically prepared according to the modified Donath and Breuner method . The preparation of hard tissue consisted of embedding in light-polymerizing 2-hydroxietyl-metacrylate. These blocks were cutting in five sections of about 200 μm and then grinding until achieving cross-sections of about 80-μm final thicknesses with an EXAKT cutting and grinding equipment (EXAKT, Norderstedt, Germany).
Bone-implant interface sections were examined under the optical microscope (Zeiss, Oberkpchen, Germany) using histological laboratory stains such as toluidine blue with Weigert haematoxylin (Merck, Kenilworth, NJ, USA) that allows the differentiation between osteoblasts and osteoclasts .
The images were processed and cross-sections were compared by means of the MIP-4 image analyser software (Digital Image Systems, SL, Barcelona) in order to quantify the bone fraction. The MIP-4 software is able to perform area and volume measurements through a computerized system connected to the optical microscope and histological lens. Area and length measurements on the images captured from the microscope were attained. All images were processed with ×10 magnification objective. The bone-to-implant contact (BIC) is calculated as the ratio of the length of the implant in contact to bone tissue and the implant perimeter, i.e. the percentage of the implant surface in contact with bone.
The quantitative results were processed with the statistical package Statgraphics plus 5.1. The significance of the differences between the groups was studied according to Student’s t test and the one-way ANOVA test (analysis of variance). p value was 0.05.
Chemical analysis by EDAX of the surface of Ti6Al4V commercial implants
Due to this process, it is unavoidable that the blasting particles induces abrasive pollution on the surface, giving rise to a surface modification not only in the final roughness but also in the chemical composition, that influences the physicochemical properties of the blasted surfaces . To minimize the drastic changes produced by of the blasting process, the posterior acid attack is usually used as a method to smooth titanium surfaces and also to eliminate the residual particles resulting from the blasting process . The use of HCl posterior to the blasting process does not assure that residual hydroxyapatite particles remain incrusted in the surface of the implants. Nevertheless, given the chemical nature of the Ca-P compounds on the surface, its presence could be even considered as beneficial in the osseointegration process.
Mean (grammes per square centimetre) and standard deviations of the bone mineral density (BMD) of tibiae and vertebral column in healthy (control) and osteoporotic (OVX) rabbits
BMD (g cm−2) tibiae
BMD (g cm−2) vertebral column
0.323 ± 0.014
0.285 ± 0.007
0.301 ± 0.016
0.271 ± 0.009
Means (grammes per square centimetre) and standard deviations of the bone mineral density (BMD) of above and below implant areas in tibiae with and without the local application of growth hormone (GH) in healthy (control) and osteoporotic (OVX) rabbits
0.356 ± 0.017
0.368 ± 0.036
0.382 ± 0.006
0.351 ± 0.021
0.366 ± 0.008
0.372 ± 0.029
0.374 ± 0.031
0.366 ± 0.015
0.308 ± 0.024
0.348 ± 0.019
0.357 ± 0.053
0.345 ± 0.027
0.369 ± 0.027
0.343 ± 0.011
0.363 ± 0.032
0.330 ± 0.024
BMD values indicate that there are no significant statistical differences either above or below the implant areas, in metaphysis and diaphysis regions, independently on the variables studied: type of implant (commercial or modified) and addition of GH local administration in the implantation site.
In agreement with the BMD results, the BIC values show no significant statistical differences independently on the local administration of GH in the implantation site and previous oxidation treatment of the implant.
A good preparation of the implant surface in order to accommodate bone topographical features contributes to accelerate the assembly between the new bone formed and the metallic implant. Research has been consequently focused on the surface modifications of implants aimed to simulate the size of the proteins or cell membrane receptors. In vitro results about the influence of different micro-nanoscale roughness on the osteoblast differentiation are sometimes contradictory [29, 30]. This is probably due to the differences between the types of cells and the types of nanoscale surface modifications used in these experiments . So, the definitive confirmation should be given by in vivo studies. In this work, the in vivo study about the use of oxidation treatments to modify the nanoroughness on the previous micro-scale roughness of the implant surface has proved to accelerate the osseointegration process.
The morphometric measurement of the BIC of osseointegrated implants is the standard procedure for the evaluation of bone formation on an implant surface. High BIC values are considered to be a prerequisite for implant stability, which clinically enables functional dental reconstruction. Studies evaluating new implant surfaces assess this parameter. In particular, differences in BIC between test and reference surfaces are statistically analysed to compare their osteogenic potential. Nevertheless, it is interesting to remark that the use of two (or even only one) histological sections per implant may strongly influence the determined BIC .
In our work, densitometric and morphometric studies point to a better bone response to the Ti6Al4V commercial implants thermally treated at 700 °C for 1 h (Figs. 5 and 6). The highest BIC value achieved for the thermally treated implant after 30 days of implantation (especially in the OVX rabbit group) could be explained by considering different features on the oxidized surface such as chemical composition and topographical properties. The chemical composition of the oxidized surface after heat treatment at 700 °C for 1 h, verified by XRD, is rutile , which is formed on the free-particle areas of the Ti6Al4V surface. Rutile scale has been proved to enhance the osteoblast response , improve the resistance to pitting corrosion  and decrease the ion release of the Ti6Al4V .
In addition, the morphology of the hard rutile scale grown on the implant surface increases nanoroughness (Fig. 4). Studies carried out by Webster et al.  have pointed out the importance of the surface roughness at the nanometre range in the connectivity to bone. It has been discussed that the increase of micro- and submicro-scale surface roughness, with feature sizes comparable to those of resorption pits of bone and cell dimensions, leads to enhanced osteoblasts differentiation and increased bone-to-implant contact in vivo .
In the specific case of osteoporotic rabbits, the results showed that the modification of the surface by the thermal treatment gives rise to a better bone response in BMD and BIC values at longer time of implantation, i.e., 30 days (Figs. 5 and 6). These results seem to indicate that the crystallography and the chemical composition given by the rutile enhance the interaction between osteoblasts and surface improving the bone regeneration around the Ti6Al4V implants.
With respect to local administration of GH to the osteoporotic rabbits, significant results have not been obtained, although a slight improvement was observed. In our study, densitometric results related to those animals in the GH treated group that were sacrificed after 15 days showed a tendency towards increased bone mineral density (BMD) that did not reach statistical significance. Our results emphasize the idea of the variability in the response to GH because, by itself, topical administration gives rise to very different results probably due to additional characteristics that affect to variables such as the host, the methodology of administration of GH or the implant itself. These results are in agreement with the authors’ previous data  and other authors . For example, Calvo-Guirado et al.  found topical application of 4 IU of GH like biomimetic agent at the moment of implant placement has no significant effects on the BIC at 5 and 8 weeks, although bone formation and inter-thread bone values did increase significantly. However, controversial about the efficiency of the topical administration of GH is found in the literature. Munoz et al.  found that topical application of growth hormone GH and melatonin synergistically enhance new bone formation around titanium implants in early stages of healing.
During the first period of 15 days, the rabbit biokinetics is appropriate to initiate a formation of young bone, which can be confirmed or not, at 30 days. In this animal model, the bone formation can be initiated before 15 days, as has been seen in other studies, but it is very spars. Moreover, the first days guide us towards an evolution of the bone response that is confirmed at 15 days. It has been published in previous works  that the fast periosteal response found could be explained by direct action of GH on the pluripotential mesenchymal cells in the first steps of the repair process. The GH accelerated this process in what has been called the “impulse effect” stimulating osteoblasts, chondroblasts, and fibroblasts. However, the most authors have not statistically found a response to GH dependent dose [10, 12], asseveration that is in accordance with our data.
Systemic and local administration of growth factors accelerates bone regeneration  and promotes osteoinductive effects . In fact, the systemic administration of GH has shown to accelerate fracture healing  at longer periods of implantation. The beneficial role of GH on the bone regeneration could be achieved at initial local administration of GH in the implantation site where oxidized Ti6Al4V implant is located and after a critical period of implantation time, systemic administration by means of small regular dose, according to .
In summary, oxidation treatments of Ti6Al4V dental implants stimulate a better bone response at longer implantation times. The local application of GH on the implantation site showed no significant effect in the osseointegration process (from BMD and BIC measurements) of thermal and commercial Ti6Al4V dental implants during the first month of implantation.
The authors acknowledge the source of funding received from Ministerio de Economia y Competitividad (Spain) through the MAT2011-29152-C02-01 project.
Availability of data and materials
Data supporting will be available in digital.csic.es repository.
Oscar G. Bodelón, Celia Clemente, Miguel Angel Alobera, Soledad Aguado-Henche, María Lorenza Escudero and María Cristina García Alonso declare that they have no competing interests.
OGB participated in the design of the study, helped to the characterization of the implants, performed the statistical analysis and helped to draft the manuscript. CC helped to the surgery and performed the analysis and interpretation of histomorphometric data. MAA carried out the surgery and helped to the interpretation of data. SAH carried out the densitometric tests and helped to the analysis and interpretation of densitometric data. MLE participated in the design of the study, coordination of tests and helped to draft the manuscript. MCGA participated in the design of the study, characterization of the implants, carried out the coordination of results and headed the draft the manuscript. All authors read and approved the final manuscript.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Lomholt TC, Pantleon K, Somers MAJ. In-vivo degradation mechanism of Ti-6Al-4V hip joints. Mater Sci Eng C. 2011;31:120–7.View ArticleGoogle Scholar
- Wisbey A, Gregson PJ, Peter LM, et al. Effect of surface treatment on the dissolution of titanium-based implant materials. Biomaterials. 1991;12:470–3.View ArticlePubMedGoogle Scholar
- Chen G, Wen X, Zhang N. Corrosion resistance and ion dissolution of titanium with different surface microroughness. Biomed Mater Eng. 1998;8:61–74.PubMedGoogle Scholar
- Garcia-Alonso MC, Saldana L, Valles G, et al. In vitro corrosion behaviour and osteoblast response of thermally oxidised Ti6Al4V alloy. Biomaterials. 2003;24:19–26.View ArticlePubMedGoogle Scholar
- Saldaña L, Barranco V, García-Alonso MC, et al. Concentration-dependent effects of titanium and aluminium ions released from thermally oxidized Ti6Al4V alloy on human osteoblasts. J Biomed Mater Res. 2006;77A:220–9.View ArticleGoogle Scholar
- Saldaña L, Vilaboa N, Vallés G, et al. Osteoblast response to thermally oxidized Ti6Al4V alloy. J Biomed Mater Res. 2005;73A:97–107.View ArticleGoogle Scholar
- Zhang L, Wu K, Song W, et al. Chitosan/siCkip-1 biofunctionalized titanium implant for improved osseointegration in the osteoporotic condition. Scientific Reports. 2015;5:10860.View ArticlePubMedPubMed CentralGoogle Scholar
- Kammerer PW, Lehnert M, Al-Nawas B, et al. Osseoconductivity of a specific streptavidin-biotin-fibronectin surface coating of biotinylated titanium implants - a rabbit animal study. Clin Implant Dent Relat Res. 2015;17 Suppl 2:e601–12.View ArticlePubMedGoogle Scholar
- Germanier Y, Tosatti S, Broggini N, et al. Enhanced bone apposition around biofunctionalized sandblasted and acid-etched titanium implant surfaces A histomorphometric study in miniature pigs. Clin Oral Impl Res. 2006;17:251–7.View ArticleGoogle Scholar
- Tresguerres IF, Clemente C, Donado M, et al. Local administration of growth hormone enhances periimplant bone reaction in an osteoporotic rabbit model. An histologic, histomorphometric and densitometric study. Clin Oral Impl Res. 2002;13:631–6.View ArticleGoogle Scholar
- Tresguerres IF, Blanco L, Clemente C, et al. Effects of local administration of growth hormone in periimplant bone: an experimental study with implants in rabbit tibiae. Int J Oral Maxillofac Implants. 2003;18:807–11.PubMedGoogle Scholar
- Tresguerres IF, Alobera MA, Baca R, et al. Histologic, morphometric, and densitometric study of peri-implant bone in rabbits with local administration of growth hormone. Int J Oral Maxillofac Implants. 2005;20:193–202.PubMedGoogle Scholar
- Lynch S, Buser D, Hernández RA, et al. Effects of the platelet derived growth factor insulin-like growth factor-I combination on bone regeneration around titanium dental implants. Results of a pilot study in beagle dogs. J Periodontol. 1991;62:710–6.View ArticlePubMedGoogle Scholar
- Calvo-Guirado JL, Mate-Sanchez J, Delgado-Ruiz R, et al. Effects of growth hormone on initial bone formation around dental implants: a dog study. Clin Oral Impl Res. 2011;22:587–93.View ArticleGoogle Scholar
- Oryan A, Alidadi S, MoshirI A, et al. Bone morphogenetic proteins: a powerful osteoinductive compound with non-negligible side effects and limitations. Biofactors. 2014;40:459–81.View ArticlePubMedGoogle Scholar
- Becker W, Linch SE, Lekholm U, et al. A comparison of e-PTFE membranes alone or in combination with platelet-derived growth factors and insulin-like growth factor-I or demineralized freeze-dried bone in promoting bone formation around immediate extraction socket implants. Periodontol. 1992;63:929–40.View ArticleGoogle Scholar
- Bak B, Andreassen TT. The effect of growth hormone on fracture healing in old rats. Bone. 1991;12:151–4.View ArticlePubMedGoogle Scholar
- Andreassen TT, Jorgensen PH, Flyvbjerg A, et al. Growth hormone stimulates bone formation and strength of cortical bone in aged rats. J Bone Miner Res. 1995;10:1057–67.View ArticlePubMedGoogle Scholar
- European Parliament and Council. Council Directive 86/609/EEC of 24 November 1986 on the protection of animals used for experimental and other scientific purposes. Official J Eur Communities. 1986;L358:1–28.Google Scholar
- Committee on Animal Nutrition; Board on Agriculture and Renewable Resources; National Research Council. Nutrient Requirements of Rabbit. 2nd rev. ed. Washington DC: National Academic of Sciences; 1977.Google Scholar
- Vidigal Jr GM, Groisman M, Gregorio LH, et al. Osseointegration of titanium alloy and HA-coated implants in healthy and ovariectomized animals: a histomorphometric study. Clin Oral Impl Res. 2009;20:1272–7.View ArticleGoogle Scholar
- Martin-Monge E, Tresguerres IF, Blanco L, et al. Validation of an osteoporotic animal model for dental implant analyses: an in vivo densitometric study in rabbits. Int J Oral Maxillofac Implants. 2011;26:725–30.PubMedGoogle Scholar
- Donath K, Breuner G. A method for the study of undecalcified bones and teeth with attached soft tissues. J Oral Pathol. 1982;11:318–26.View ArticlePubMedGoogle Scholar
- Chappard D, Baslé MF, Legrand E, et al. New laboratory tools in the assessment of bone quality. Osteoporos Int. 2011;22:2225–40.View ArticlePubMedGoogle Scholar
- Barranco V, Escudero ML, Garcia-Alonso MC. 3D, chemical and electrochemical characterization of blasted Ti6Al4V surfaces: Its influence on the corrosion behavior. Electrochim Acta. 2007;52:4374–84.View ArticleGoogle Scholar
- Diniz MG, Soares GA, Coelho MJ, et al. Surface topography modulates the oeteogenesis in human bone marrow cell cultures grown on titanium samples prepared by a combination of mechanical and acid treatments. J Mater Sci. 2002;13:421–32.Google Scholar
- Barranco V, Onofre E, Escudero ML, et al. Characterization of roughness and pitting corrosion of surfaces modified by blasting and thermal oxidation. Surf Coat Tech. 2010;204:3783–93.View ArticleGoogle Scholar
- Billi F, Onofre E, Ebramzadeh E, et al. Characterization of modified Ti6Al4V alloy after fretting–corrosion tests using near-field microscopy. Surf Coat Tech. 2012;212:134–44.View ArticleGoogle Scholar
- Webster TJ, Ejiofor JU. Increased osteoblasts adhesion on nanophase metals: Ti. Ti6Al4V and CoCrMo. Biomaterials. 2004;25:4731–9.View ArticlePubMedGoogle Scholar
- Cai KY, Bossert J, Jandt KD. Does the nanometer scale topography of titanium influence protein adsorption and cell proliferation? Colloids Surf B: Biointerfaces. 2006;49:136–44.View ArticlePubMedGoogle Scholar
- Gittens RA, McLachlan T, Olivares-Navarrete R, et al. The effects of combined micron-submicron scale surface roughness and nanoscale features on cell proliferation and differentiation. Biomaterials. 2011;32:3395–403.View ArticlePubMedGoogle Scholar
- Bernhardt R, Kuhlisch E, Schulz MC, et al. Comparison of bone-implant contact and bone-implant volume between 2d-histological sections and 3D-SR-μCT slices. Eur Cells Mater. 2012;23:237–48.Google Scholar
- Cochran DL, Schenk RK, Lussi A, et al. Bone response to unloaded and loaded titanium implants with a sandblasted and acid-etched surface: a histometric study in the canine mandibule. J Biomed Mater Res. 1998;40:1–11.View ArticlePubMedGoogle Scholar
- Lutz R, Srour S, Nonhoff J, et al. Biofunctionalization of titanium implants with a biomimetic active peptide (P-15) promotes early osseointegration. Clin Oral Imp Res. 2010;21:726–34.View ArticleGoogle Scholar
- Muñoz F, López-Peña M, Miño N, et al. Topical application of melatonin and growth hormone accelerates bone healing around dental implants in dogs. Clin Oral Imp Res. 2012;14:226–35.View ArticleGoogle Scholar
- Raschke MJ, Bail H, Windhagen HJ, et al. Recombinant growth hormone accelerates bone regenerate consolidation in distraction osteogenesis. Bone. 1999;24:81–8.View ArticlePubMedGoogle Scholar
- Schmidmaier G, Wildemann B, Bail H, et al. Local application of growth factors (insulin-like growth factor-1 and transforming growth factor-β1) from a biodegradable poly(D, L-lactide) coating of osteosynthetic implants accelerates fracture healing in rats. Bone. 2001;28:341–50.View ArticlePubMedGoogle Scholar
- Schmidmaier G, Wildemann B, Heeger J, et al. Improvement of fracture healing by systemic administration of growth hormone and local application of insulin-like growth factor-1 and transforming growth factor-β1. Bone. 2002;31:165–72.Google Scholar